**Technology of Thermal Treatment**

Using large pellets for the processing of strontium aluminate clinker (Fig.31 in Chapter 4.5) may change the behaviour during thermal treatment as well as some properties of the prod‐ uct due to increasing influence of partial pressure of carbon dioxide on the thermal decom‐ position of strontium carbonate. The material forming the diffusion barrier as the reaction zone is shifted from the surface into the deeper zones of pellet. Increasing partial pressure of carbon dioxide slows down the rate of thermal decomposition of strontium carbonate and increases the temperature required for the thermal decomposition (please see the discussion in Chapter 4.2) and temporary lack of SrO in the reaction zone. Therefore, the influence of large pellets on prepared strontium aluminate clinker is similar to the usage of mixture with

84 Strontium Aluminate - Cement Fundamentals, Manufacturing, Hydration, Setting Behaviour and Applications

lower saturation degree (discussed in Chapter 4).

Cement is made of clinker and ground gypsum, whereas clinker is produced from fired limestone and clay mixed in particular percentages. Portland cement clinker was first made in 1842 in modified form of traditional static limekiln. Around 1885, the experiments began on the design of continuous kilns. One of the designs was the shaft kiln, similar in design to a blast furnace. The raw meal in the form of lumps and fuel were continuously added at the top, and clinker was continually withdrawn at the bottom. Compressed air was blown through from the base to combust the fuel. The shaft kiln had been used for only short period of time before it was forced out by the rotary kiln, but it has had a limited renaissance from 1970 onward in China and elsewhere, when it has been used for the small-scale, low-tech plants in rural areas away from transport access. A typical shaft kiln can produce 100–200 tons/day. Nowadays, rotary kiln is one of the key equipment in cement industry used to convert calcineous raw meal to cement clinker. Raw meal for the cement production is a mixture of predetermined proportions of limestone, silica, and small quantities of alumina and iron oxide [295,296].

The cement making processes are extremely energy consuming. Typically for the production of one ton of cement, a well-equipped plant consumes nearly 3 GJ. For each ton of produced clinker an equivalent amount of greenhouse gases is emitted. The manufacture of cement is the focus of considerable attention worldwide because of giant amount of used energy and high environmental impact of the process. Considering the recent impetus on the emission of greenhouse gases reductions and on the reduction of energy consumption, a renewed emphasis arises on developing the computational models for cement industry and on applying this understanding for the performance enhancement [297].

The most important plant unit in cement manufacturing is the kiln [298]. The raw material passes sequentially through pre-heater, calciner, kiln and cooler to form the cement clinker. In a pre-heater section the raw meal is pre-heated to the calcination temperature via hot gases coming from calciner. In calciner, the raw meal is partially calcined. The energy required for the endothermic calcination reaction is provided by combusting a suitable fuel. In most cases, coal is used to provide the required energy, especially in India. The calciner is supplied with tertiary air from the cooler and with air coming out of kiln exhaust. The former is to supply coal with O2 sufficiently during the combustion and the later to utilize the heat of kiln gases to enhance the calcination reaction. Hot gases from calciner are sent to pre-heater assembly to pre-heat the solids. Partially calcined solids from the calciner are fed slowly to a rotary kiln. In rotary kiln, remaining calcination and other reactions of formation of clinker phases proceed [297,299,300].

© 2014 The Author(s). Licensee InTech. This chapter is distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/3.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

The energy required for the endothermic clinker reactions is provided by burning coal in the kiln. The pulverized coal along with the pre-heated air (secondary air) is fed to the kiln in a counter current mode with respect to solids. A part of solids melts in the kiln. The melt causes an internal coating on the kiln refractory. The counter current flow of gas entrains solid particles in the free board region. Such entrainment enhances the rates of radiative heat transfer by increasing effective emissivity and conductivity. Hot clinker is discharged from kiln to clinker cooler and hot gases from kiln exhaust are sent to the calciner. In clinker cooler, a part of energy of solids is recovered back by heat exchange with air. The pre-heated air from coolers is passed to kiln and calciner as secondary and tertiary air, respectively. A small part of air may be vented if required [297].

The heating rate does not play so important role during the processing of strontium aluminate clinker such as for Portland cement, where the decomposition of tricalcium silicate to dicalcium silicate and free water and the formation of *γ*-dicalcium silicate threaten to devalue the binding properties. On the other hand, increasing cooling rate increases the reactivity of glass phase.

Technology of Thermal Treatment 87

The processes which take place during the thermal treatment of raw meal to strontium

**1.** Drying: evaporation of free and physically bonded water and adsorbed water without the changes of chemical composition of dry mater. Drying is usually finished up to the

**2.** Dehydroxylation: thermal treatment of aluminium hydroxide; water is released from

**4.** Formation of strontium aluminate and the establishment of equilibrium composition.

Drying is the technological process, which removes water from treated material by evapora‐ tion. Therefore, the reduction of material moisture does not usually relate to the significant changes in mineralogical composition, the raw material is often considered as the two-

In the dryer, water evaporates from material to flow of air, but the amount of water that can be absorbed by gas phase depends on the conditions of drying process. If the gas phase is supersaturated by water at given temperature, the moisture of material does not decrease any

There is certain value of maximum amount of water that can be absorbed by air at constant temperature and pressure. Therefore, three parameters are necessary for the characterization

**•** Temperature (*T*): the maximum amount of water that can be absorbed by gas phase increases

more. Therefore, the drying process must respect certain physical regularities.

**•** Moisture: can be characterized by several ways which are described below.

**•** To specify the content of water in air the following parameters can be used:

aluminate clinker are:

temperature of 105 ± 5 °C.

hydroxyl groups of mineral.

**5.** Sintering of solid phase.

**7.** Cooling of clinker.

**2. Drying**

of the state of air:

**•** Pressure (*P*);

with temperature.

**3.** Thermal decomposition of strontium carbonate:

**6.** Formation of melt and sintering of liquid phase.

component mixture of dry mater and water.

The clinker formation process by the fluidized bed kiln system was developed by Yuko at al. [301].The average size of clinker produced by this system is about 2 mm, that is much smaller than that of a rotary kiln clinker.

## **1. Thermal treatment of strontium aluminate clinker**

The synthesis of strontium aluminate clinker requires the raw material pre-treatment, the calculation of composition, the preparation of mixture of raw materials, the homogenization or granulation, the thermal treatment, the grinding and fine milling of strontium aluminate clinker. The individual steps of this process are discussed in this chapter. The scheme of production technology of clinker is schematically shown in Fig.1.

**Figure 1.** Scheme of clinker production technology.

The heating rate does not play so important role during the processing of strontium aluminate clinker such as for Portland cement, where the decomposition of tricalcium silicate to dicalcium silicate and free water and the formation of *γ*-dicalcium silicate threaten to devalue the binding properties. On the other hand, increasing cooling rate increases the reactivity of glass phase.

The processes which take place during the thermal treatment of raw meal to strontium aluminate clinker are:


## **2. Drying**

The energy required for the endothermic clinker reactions is provided by burning coal in the kiln. The pulverized coal along with the pre-heated air (secondary air) is fed to the kiln in a counter current mode with respect to solids. A part of solids melts in the kiln. The melt causes an internal coating on the kiln refractory. The counter current flow of gas entrains solid particles in the free board region. Such entrainment enhances the rates of radiative heat transfer by increasing effective emissivity and conductivity. Hot clinker is discharged from kiln to clinker cooler and hot gases from kiln exhaust are sent to the calciner. In clinker cooler, a part of energy of solids is recovered back by heat exchange with air. The pre-heated air from coolers is passed to kiln and calciner as secondary and tertiary air, respectively. A small part of air

86 Strontium Aluminate - Cement Fundamentals, Manufacturing, Hydration, Setting Behaviour and Applications

The clinker formation process by the fluidized bed kiln system was developed by Yuko at al. [301].The average size of clinker produced by this system is about 2 mm, that is much smaller

The synthesis of strontium aluminate clinker requires the raw material pre-treatment, the calculation of composition, the preparation of mixture of raw materials, the homogenization or granulation, the thermal treatment, the grinding and fine milling of strontium aluminate clinker. The individual steps of this process are discussed in this chapter. The scheme of

**1. Thermal treatment of strontium aluminate clinker**

production technology of clinker is schematically shown in Fig.1.

may be vented if required [297].

than that of a rotary kiln clinker.

**Figure 1.** Scheme of clinker production technology.

Drying is the technological process, which removes water from treated material by evapora‐ tion. Therefore, the reduction of material moisture does not usually relate to the significant changes in mineralogical composition, the raw material is often considered as the twocomponent mixture of dry mater and water.

In the dryer, water evaporates from material to flow of air, but the amount of water that can be absorbed by gas phase depends on the conditions of drying process. If the gas phase is supersaturated by water at given temperature, the moisture of material does not decrease any more. Therefore, the drying process must respect certain physical regularities.

There is certain value of maximum amount of water that can be absorbed by air at constant temperature and pressure. Therefore, three parameters are necessary for the characterization of the state of air:


$$W\_R = \frac{P\_D}{P\_D^\*} = \frac{W\_A}{W\_A^\*} \tag{1}$$

C+O CO 22 r ® (Δ H° = -393 484 kJ) (3)

C+1/2 O O 2 r ® C (Δ H° = -110 696 kJ) (4)

S+O CO 22 r ® (Δ H° = -296 511 kJ) (5)

) of gaseous water is formed during this process. Air used for

CH +O CO +2 H O 42 2 2 ® (7)

C+2 H (g) CH (g) 2 4 ® (8)

. Depending on the conditions the following expressions of

<sup>=</sup> *Amount of applied air or oxygen <sup>n</sup> Stoichiometric amount of applied air or oxygen* (6)

<sup>3</sup> of air are necessary for the combustion

Technology of Thermal Treatment 89

of inert N2 gas. The combustion process is termed

For these purposes, the dry air is considered as the mixture of ~21 vol. % O2 and ~79 % N2. Therefore the O2 : N2 and O2 : Air ratios are 21 : 79=1 : 3.76 and 21 : 100=1 : 4.76, respectively. Using the Avogadro law, one kmol of gaseous species under standard conditions corresponds

3

The amount of applied oxygen may be stoichiometric, higher or lower than stoichiometric. It

Depending on this, neutral (*n* ≈ 1), oxidizing (*n* > 1) or reducing conditions (*n* < 1) can occur in

The reaction enthalpy for the other species can be calculated from tabulated thermodynamic data, e.g. [303,304], or using the Kirchhoff's laws. For example, the ideal combustion of

with **Δ**r*H°*=-802 803 kJ. Therefore, the formation of methane (Eq.8) shows the reaction enthalpy

That relationship reveals that the value of **Δ**r*H°*(Eq.7)=**Δ**r*H°*(Eq.3)+2 **Δ**r*H°*(Eq.2)-**Δ**r*H°*(Eq.

Heat released by the combustion of one mol of fuel under standard conditions is termed as the

(subscript "*N*" denotes normal condition, i.e. the temperature of 273,15 K and the

to 22.4 mN

3

pressure of 0.1013 MPa).

the furnace atmosphere.

of-73 843 kJ:

8)=-802 803 kJ.

heat of combustion (**Δ**c*H*°)1

1 It stands to reason that Δr*H*° = Δc*H*° for Eqs.2 - 5 and Eq. 7.

combustion heat apply:

of 1 kmol of H2. 1 kmol (22.4 mN

For example, according to Eq.2, 0.5∙22.4∙4.76=53.3 mN

can be described by the following dimensionless ratio:

the oxidation contains 0.5∙22.4∙3.76=42.1 mN

methane gas is expressed by the equation:

3

as ideal, if the final product contains only CO2, H2O and SO2 species.


The driers use the heat of drying air phase to reduce the moisture of dried material. The temperature of air decreases as water evaporates but the formed water vapor that possesses this heat becomes the part of air phase. In the other words, if the losses aren't taken into account, the enthalpy of air is constant during the drying process. The drier without the heat losses is termed theoretical drier.

Rotary dryers are commonly used to dry and process granular materials. They are applied across a wide range of industries ranging from food production to cement production. Rotary dryers contain lifters to lift the material away from the bottom of the dryer and then to drop it through the gas to promote the mass and heat transfer between the granular material and the gaseous phase [302].

#### **3. Firing process**

Firing process includes the technology and equipment which provide heat in order to reach the temperature necessary to achieve required phase composition and properties of the product. Ceramic and concrete technology use furnaces of different type, but it is not necessary to use the pre-calcination unit as for the preparation of strontium aluminate cement. That implies from higher thermal stability of SrCO3 when compared with CaCO3 (discussed in Chapter 4.2). This turns the attention to the technologies of heat regeneration or recuperation from gas processing.

The furnace is heated by the combustion of fuel, the components of which are oxidized according to the following exothermic reactions:

$$\text{H}\_2 + \text{l}/2\text{ O}\_2 \rightarrow \text{H}\_2\text{O} \quad \text{ (}\Delta\_\text{r}\text{H}^\circ = \text{-241 581 kJ}\text{)}\tag{2}$$

$$\text{C} + \text{O}\_2 \rightarrow \text{CO}\_2 \qquad \left(\Delta\_\text{r} \text{H}^\circ = \text{-} \text{993 } 484 \text{ kJ}\right) \tag{3}$$

$$\text{C} + \text{l}/2\text{ O}\_2 \rightarrow \text{CO} \qquad \left(\Delta\_\text{r}\text{H}^\circ = \text{-l} \, 10\text{ }696\text{ kJ}\right) \tag{4}$$

$$\text{S} \text{+O}\_2 \rightarrow \text{CO}\_2 \qquad \quad \left(\Delta\_r \text{H}^\circ = \text{-296 511 kJ}\right) \tag{5}$$

For these purposes, the dry air is considered as the mixture of ~21 vol. % O2 and ~79 % N2. Therefore the O2 : N2 and O2 : Air ratios are 21 : 79=1 : 3.76 and 21 : 100=1 : 4.76, respectively. Using the Avogadro law, one kmol of gaseous species under standard conditions corresponds to 22.4 mN 3 (subscript "*N*" denotes normal condition, i.e. the temperature of 273,15 K and the pressure of 0.1013 MPa).

For example, according to Eq.2, 0.5∙22.4∙4.76=53.3 mN <sup>3</sup> of air are necessary for the combustion of 1 kmol of H2. 1 kmol (22.4 mN 3 ) of gaseous water is formed during this process. Air used for the oxidation contains 0.5∙22.4∙3.76=42.1 mN 3 of inert N2 gas. The combustion process is termed as ideal, if the final product contains only CO2, H2O and SO2 species.

The amount of applied oxygen may be stoichiometric, higher or lower than stoichiometric. It can be described by the following dimensionless ratio:

$$n = \frac{\text{Amount of applied air or oxygen}}{\text{Stoticichiometric amount of applied air or oxygen}}\tag{6}$$

Depending on this, neutral (*n* ≈ 1), oxidizing (*n* > 1) or reducing conditions (*n* < 1) can occur in the furnace atmosphere.

The reaction enthalpy for the other species can be calculated from tabulated thermodynamic data, e.g. [303,304], or using the Kirchhoff's laws. For example, the ideal combustion of methane gas is expressed by the equation:

$$\text{CH}\_4 + \text{O}\_2 \rightarrow \text{CO}\_2 + 2\text{ H}\_2\text{O} \tag{7}$$

with **Δ**r*H°*=-802 803 kJ. Therefore, the formation of methane (Eq.8) shows the reaction enthalpy of-73 843 kJ:

$$\text{C} + 2\,\text{H}\_2(\text{g}) \to \text{CH}\_4(\text{g})\tag{8}$$

That relationship reveals that the value of **Δ**r*H°*(Eq.7)=**Δ**r*H°*(Eq.3)+2 **Δ**r*H°*(Eq.2)-**Δ**r*H°*(Eq. 8)=-802 803 kJ.

Heat released by the combustion of one mol of fuel under standard conditions is termed as the heat of combustion (**Δ**c*H*°)1 . Depending on the conditions the following expressions of combustion heat apply:

**•** Partial pressure of water vapor in air (*P*D [Pa]).

meter of air.

air.

**•** Temperature of wet point (*T*wp);

termed theoretical drier.

the gaseous phase [302].

**3. Firing process**

from gas processing.

according to the following exothermic reactions:

**•** Temperature of wet thermometer (*T*wt).

**•** Absolute air humidity (*W*<sup>A</sup> [kg∙m-3]) is defined as the weight of water vapour per cubic

**•** Relative air humidity (*W*R) is defined as the dimensionless ratio of parameters mentioned

**•** Specific air humidity (*W*S [kgw∙kgair-1]) is the weight of water vapours in one kilogram of dry

The driers use the heat of drying air phase to reduce the moisture of dried material. The temperature of air decreases as water evaporates but the formed water vapor that possesses this heat becomes the part of air phase. In the other words, if the losses aren't taken into account, the enthalpy of air is constant during the drying process. The drier without the heat losses is

Rotary dryers are commonly used to dry and process granular materials. They are applied across a wide range of industries ranging from food production to cement production. Rotary dryers contain lifters to lift the material away from the bottom of the dryer and then to drop it through the gas to promote the mass and heat transfer between the granular material and

Firing process includes the technology and equipment which provide heat in order to reach the temperature necessary to achieve required phase composition and properties of the product. Ceramic and concrete technology use furnaces of different type, but it is not necessary to use the pre-calcination unit as for the preparation of strontium aluminate cement. That implies from higher thermal stability of SrCO3 when compared with CaCO3 (discussed in Chapter 4.2). This turns the attention to the technologies of heat regeneration or recuperation

The furnace is heated by the combustion of fuel, the components of which are oxidized

H +1/2 O H O ( 1 581 ) kJ 2 22 r ® Δ H° = -24 (2)

\* or *W*<sup>A</sup> \* ):

*P W* (1)

above for actual state of air (*P*D or *W*A) and air supper saturated by water (*P*<sup>D</sup>

88 Strontium Aluminate - Cement Fundamentals, Manufacturing, Hydration, Setting Behaviour and Applications

\* \* = = *D A <sup>R</sup> D A P W <sup>W</sup>*

<sup>1</sup> It stands to reason that Δr*H*° = Δc*H*° for Eqs.2 - 5 and Eq. 7.

**a.** Higher Heating Value (HHV) or High Caloric Value (HCV): heat released during ideal combustion process performed under standard ambient conditions2 . Formed products were cooled to their original temperature, i.e. the temperature before combustion. All formed water vapor condensed to liquid. For example:

$$\text{CH}\_4(\text{g}) + \text{O}\_2(\text{g}) \rightarrow \text{CO}\_2(\text{g}) + 2\text{ H}\_2\text{O}(\text{l}) \qquad \text{HHV} = 890 \text{ 564 kJ} \cdot \text{mol}^{-1} \tag{9}$$

**Fuel Coal Oil Gas**

C 89.0 87,5 --- H2 5.0 11 0,4 S 1 0,8 --- N2 3 0,5 2,5 CO2 --- --- 1,6 CH4 --- --- 95.5 SiO2 2 --- ---

**Table 2.** Composition of coal, oil and gas applied for calculation.

be seen from Fig.2.

Species Composition [wt.%] Composition [vol.%]

Technology of Thermal Treatment 91

The content of SrO was recalculated to SrCO3 via the multiplication by MSrCO3/MSrO ratio (147.63/ 103.62=1.42). Other admixtures are neglected and the raw mixture composition is recalculated

Assuming the composition mentioned above, the raw material feed of 100 tons per hour, coal used as a fuel to keep the process temperature of 1250 °C and the content of strontium aluminate in clinker at least 90 %, the calculated material and energetic balance of furnace can

**Figure 2.** An example materials (a) and enthalpy balance (b) for the strontium aluminate clinker preparation process.

to 100 % as is shown in Table 1. The composition of coal is given by Table 2.

**b.** Lower Heating value (LHV), Lower Caloric Value (LCV) or Net Caloric Value (NCV): similar to HHV, but water produced by the combustion process stays in gas phase (Eq. 10). It is obvious that HHV and LHV differ in the enthalpy related to the condensation of water-44 kJ∙mol-1. For two mols of water the difference HHV(Eq.9) – LHV(Eq.10)=-88 kJ∙mol-1, i.e. HHV=LHV+latent heat of water.

$$\text{CH}\_4(\text{g}) + \text{O}\_2(\text{g}) \rightarrow \text{CO}\_2(\text{g}) + 2\text{H}\_2\text{O}(\text{g}) \qquad \text{LHV} = \text{802.556 kJ} \cdot \text{mol}^{-1} \tag{10}$$

The bomb calorimeter is used for the determination of heating values of fuels.

The physicochemical environment of cement kilns is ideal for the co-combustion of a number of organic wastes. The economic, as well as environmental benefits are achieved by the substitution of fossil fuels, mainly coal and petcoke. Specific types of alternative fuels (AFs) derived from the mixtures of wastes, such as animal byproduct waste (ABW), agricultural plastic waste (APW), automotive waste plastics (AWP), biological sludge (BIS), cutting oil emulsions (COI), cable plastic waste (CPW), demolition waste (DW), industrial waste fuel (INBRE), refuse derived fuel (RDF or BRAM or SRF), rice husk (RH), refinery sludge (RS), spent solvents (SS), tire derived fuel (TDF), waste oils (WO), etc., are developed [305-308].


**Table 1.** The composition of raw meal.

Adopting the raw material composition from Fig.1 (calculated for *M*H=0.98 as was described in Chapter 2.3.1), it is possible to provide the example for calculation of material and energetic balance for the process of calcination of strontium aluminate clinker.

<sup>2</sup> The standard temperature and pressure conditions (STP, 0°C and 100 kPa) are different from standard ambient temperature and pressure (SATP, 25 °C and 100 kPa).


**Table 2.** Composition of coal, oil and gas applied for calculation.

**a.** Higher Heating Value (HHV) or High Caloric Value (HCV): heat released during ideal

**b.** Lower Heating value (LHV), Lower Caloric Value (LCV) or Net Caloric Value (NCV): similar to HHV, but water produced by the combustion process stays in gas phase (Eq. 10). It is obvious that HHV and LHV differ in the enthalpy related to the condensation of water-44 kJ∙mol-1. For two mols of water the difference HHV(Eq.9) – LHV(Eq.10)=-88

The physicochemical environment of cement kilns is ideal for the co-combustion of a number of organic wastes. The economic, as well as environmental benefits are achieved by the substitution of fossil fuels, mainly coal and petcoke. Specific types of alternative fuels (AFs) derived from the mixtures of wastes, such as animal byproduct waste (ABW), agricultural plastic waste (APW), automotive waste plastics (AWP), biological sludge (BIS), cutting oil emulsions (COI), cable plastic waste (CPW), demolition waste (DW), industrial waste fuel (INBRE), refuse derived fuel (RDF or BRAM or SRF), rice husk (RH), refinery sludge (RS), spent solvents (SS), tire derived fuel (TDF), waste oils (WO), etc., are developed [305-308].

were cooled to their original temperature, i.e. the temperature before combustion. All



**[%] wt. [g] [%] wt. [%] mol.**

**Raw mixture after recalculation**

. Formed products

combustion process performed under standard ambient conditions2

90 Strontium Aluminate - Cement Fundamentals, Manufacturing, Hydration, Setting Behaviour and Applications

The bomb calorimeter is used for the determination of heating values of fuels.

**Constituents**

balance for the process of calcination of strontium aluminate clinker.

SrO 49.1 SrCO3 70.0 58.3 49.3 Al2O3 49.2 Al2O3 49.2 41.0 50.2 Fe2O3 0.9 Fe2O3 0.9 0.7 0.6 Σ 99.2 Σ 120.1 100 100

Adopting the raw material composition from Fig.1 (calculated for *M*H=0.98 as was described in Chapter 2.3.1), it is possible to provide the example for calculation of material and energetic

2 The standard temperature and pressure conditions (STP, 0°C and 100 kPa) are different from standard ambient

formed water vapor condensed to liquid. For example:

kJ∙mol-1, i.e. HHV=LHV+latent heat of water.

**Raw mixture**

**Table 1.** The composition of raw meal.

temperature and pressure (SATP, 25 °C and 100 kPa).

**Constituents**

The content of SrO was recalculated to SrCO3 via the multiplication by MSrCO3/MSrO ratio (147.63/ 103.62=1.42). Other admixtures are neglected and the raw mixture composition is recalculated to 100 % as is shown in Table 1. The composition of coal is given by Table 2.

Assuming the composition mentioned above, the raw material feed of 100 tons per hour, coal used as a fuel to keep the process temperature of 1250 °C and the content of strontium aluminate in clinker at least 90 %, the calculated material and energetic balance of furnace can be seen from Fig.2.

**Figure 2.** An example materials (a) and enthalpy balance (b) for the strontium aluminate clinker preparation process.

The presence of silica in raw materials or coal used as the fuel may lead to the formation of mullite and strontium bearing feldspar3 . Both are non-reactive temperature stable compounds without hydraulic behaviour but may serve as microfiller. The reaction of the process which takes place during the calcination of strontium aluminate clinker is discussed in Chapter 4.

Based on the discussion in Chapter 6.1.5, heating to the temperature interval of recrystallization of SrA phase (1300 – 1400 °C) seems to be the optimal conditions for the processing of strontium aluminate clinker. The formation of large crystals due to increasing temperature of thermal treatment over 1400 °C is undesirable since the reactivity of strontium aluminate clinker decreases and the cost of production increases. The sintering and formation of glassy phase at the temperatures over 1450°C (Chapter 4.3.3) increase the demands on grinding of calcinate

Hot solids from the kiln are discharged on the grate of clinker cooler. As the grate moves with uniform speed along the cooler length, the solids lose their heat in cross-flow air. First part of air is generally sent to the kiln as secondary air, second part to calciner as tertiary air and third part is vented to the surroundings (vent air). The clinker comes out of the rotary kiln having high temperature of 1380 °C and is cooled by fresh incoming air to the temperature of 65 °C

**i.** Supplies the kiln with desired quantity of secondary air at correct pressure and

**ii.** Fast cooling the clinker to prevent any further reactions, and far enough to permit

The effect of OPC cooling rate on the fluidity of mortars was investigated by Nakano at al. [309]. The C4AF crystallite size calculated by the Rietveld method can be used to measure the cooling rate of clinker and to predict the fluidity of mortar. The fluidity of mortar increased with increasing cooling rate and with decreasing C3A content. In slowly cooled clinker the calcium aluminoferrite phase is definitely lower in amount and Al2O3/Fe2O3 ratio than in rapidly cooled clinker [310]. Fast cooling rate results in the higher hydraulic reactivity of

Rotary kilns produce an intermediate product called "clinker." Clinker is ground to produce cement [311]. More finely ground cement has larger specific surface and the reactive area available for the reaction with water is thus larger. The contact between surfaces of fine additives and sand is improved as well, the initial hydration of clinker minerals is made easier, and the distribution of hydration products is accelerated. It is recommended to keep the

to reach the optimal cement properties. Small addition of gypsum or anhydrite retards the

g-1 if we want

Technology of Thermal Treatment 93

particle fineness expressed by the specific surface in the range of 2150–2400 cm2

(Chapter 3.5).

[297,299].

**4. Cooling of clinker**

temperature.

**5. Grinding of clinker**

start of cement sludge setting [312-315].

further handling.

The clinker cooler serves for two purposes [298]:

cement and reduce the setting time of cement slurry [1010].

Using oil or gas (Table 2) under the same conditions and kiln charge leads to the enthalpy balance shown in Fig.3.

**Figure 3.** Preparation of strontium aluminate clinker using oil and gas as the fuel.

<sup>3</sup> These feldspars have general composition given by formula Me2+Al2Si2O8, where Me2+ = Ca2+, Sr2+ and Ba2+. Calcium, strontium and barium bearing feldspars are known as minerals anorthite, slawsonite ((Sr,Ca)Al2Si2O8, sometimes termed as Sr-celsian [893,901]) and celsian, respectively. The crystallization of celsian is studied for the preparation of celsian ceramics and glass ceramics [893,895,901]. The formation of celsian was observed by Rezaie at al [15] after the addition of 10 % colloidal silica or kaolin to barium aluminate cement. Regardless the source, the addition of SiO2 increases the setting time, improves workability and mechanical properties.

Based on the discussion in Chapter 6.1.5, heating to the temperature interval of recrystallization of SrA phase (1300 – 1400 °C) seems to be the optimal conditions for the processing of strontium aluminate clinker. The formation of large crystals due to increasing temperature of thermal treatment over 1400 °C is undesirable since the reactivity of strontium aluminate clinker decreases and the cost of production increases. The sintering and formation of glassy phase at the temperatures over 1450°C (Chapter 4.3.3) increase the demands on grinding of calcinate (Chapter 3.5).

## **4. Cooling of clinker**

The presence of silica in raw materials or coal used as the fuel may lead to the formation of

92 Strontium Aluminate - Cement Fundamentals, Manufacturing, Hydration, Setting Behaviour and Applications

without hydraulic behaviour but may serve as microfiller. The reaction of the process which takes place during the calcination of strontium aluminate clinker is discussed in Chapter 4.

Using oil or gas (Table 2) under the same conditions and kiln charge leads to the enthalpy

**Figure 3.** Preparation of strontium aluminate clinker using oil and gas as the fuel.

setting time, improves workability and mechanical properties.

3 These feldspars have general composition given by formula Me2+Al2Si2O8, where Me2+ = Ca2+, Sr2+ and Ba2+. Calcium, strontium and barium bearing feldspars are known as minerals anorthite, slawsonite ((Sr,Ca)Al2Si2O8, sometimes termed as Sr-celsian [893,901]) and celsian, respectively. The crystallization of celsian is studied for the preparation of celsian ceramics and glass ceramics [893,895,901]. The formation of celsian was observed by Rezaie at al [15] after the addition of 10 % colloidal silica or kaolin to barium aluminate cement. Regardless the source, the addition of SiO2 increases the

. Both are non-reactive temperature stable compounds

mullite and strontium bearing feldspar3

balance shown in Fig.3.

Hot solids from the kiln are discharged on the grate of clinker cooler. As the grate moves with uniform speed along the cooler length, the solids lose their heat in cross-flow air. First part of air is generally sent to the kiln as secondary air, second part to calciner as tertiary air and third part is vented to the surroundings (vent air). The clinker comes out of the rotary kiln having high temperature of 1380 °C and is cooled by fresh incoming air to the temperature of 65 °C [297,299].

The clinker cooler serves for two purposes [298]:


The effect of OPC cooling rate on the fluidity of mortars was investigated by Nakano at al. [309]. The C4AF crystallite size calculated by the Rietveld method can be used to measure the cooling rate of clinker and to predict the fluidity of mortar. The fluidity of mortar increased with increasing cooling rate and with decreasing C3A content. In slowly cooled clinker the calcium aluminoferrite phase is definitely lower in amount and Al2O3/Fe2O3 ratio than in rapidly cooled clinker [310]. Fast cooling rate results in the higher hydraulic reactivity of cement and reduce the setting time of cement slurry [1010].

## **5. Grinding of clinker**

Rotary kilns produce an intermediate product called "clinker." Clinker is ground to produce cement [311]. More finely ground cement has larger specific surface and the reactive area available for the reaction with water is thus larger. The contact between surfaces of fine additives and sand is improved as well, the initial hydration of clinker minerals is made easier, and the distribution of hydration products is accelerated. It is recommended to keep the particle fineness expressed by the specific surface in the range of 2150–2400 cm2 g-1 if we want to reach the optimal cement properties. Small addition of gypsum or anhydrite retards the start of cement sludge setting [312-315].

The procedure is divided into two sequential phases; crushing of lumps (3 – 25 mm) into loosely connected wafers in a dry roller press and subsequent fine milling of pre-processed clinker wafers in a rotating ball mill [316].

cined bauxite and alumina can be introduced into the clinker. These mineral admixtures serve as micro-fillers, similarly to calcite4 milled with clinker during the preparation of Port‐ land cement [315,320,323,324]. The grinding kinetics, the effect of grinding media and the

Technology of Thermal Treatment 95

4 The use of Portland limestone cements has many benefits, both technical and economical. The European Prestandard prEN 197-1 identifies two types of Portland limestone cement containing 6–20% limestone and 21–35% limestone,

respectively [320].

additives were already described in Chapter 2.7.

As was mentioned above, the ball mill is commonly used for fine milling of cement clinkers. The type of grinding media exerts significant influence on milling performance in terms of the product size and energy consumption. Various shapes of grinding media including rods, pebbles, and cylinders are used as an alternative to balls. The cylinders received particular attention because they have a greater surface area and higher bulk density than balls of similar mass and size [317-320].

Grinding of clinker represents energetically demanding part of the production process, which consumes about one-third of energy needed to produce cement. The production of fine ground clinker requires grinding stabilizers (grinding activators) which prevent the clinker from reagglomeration. Such additives, which are well known in both dry grinding and wet grinding processes, help decrease the enormous energy consumption of cement production [285,313,321].

For most of the twentieth century, the dry grinding circuits for the production of finished cement from cement clinker which consist of two-compartment tube mills and air separators, have been used. It is not uncommon to produce cement in an open circuit. The advances in cement grinding technology are slow and limited to more developed countries. Approximately 95% of feed to the cement grinding circuit are clinker and the rest of feed are ''additives'' which include grinding aids. The quality of cement is measured by the surface area or the Blaine index. The unit of the Blaine index is m2 /kg, and this index is determined by the Blaine air permeability test. In the past 20 years, high pressure grinding roll (HPGR) technology has been used in pre-crushing the clinker. Presently, many American and European cement grinding circuits have HPGR which increases the grinding capacity and energy efficiency [279].

The effectiveness of seven grinding aids, namely triethanolamine, mono-and diethylene glycols, oleic acid, sodium oleate, sulphite waste liquor and dodecylbenzene sulphonic acid on the batch grinding of Portland cement clinker, limestone and quartz was investigated in a laboratory ball mill by Sohoni at al. [322]. While the grinding aids had only a marginal effect on grinding of quartz, they had significantly beneficial effect on the grinding of limestone and cement clinker. Triethanolamine appeared to be the most effective of all aids studied. In grinding of cement clinker, gypsum also acted as very effective grinding aid. The action of these additives was attributed to their ability to prevent the agglomeration and balls and mill from coating by powder.

The presence of easily ground limestone leads to a wider particle size distribution of mixture. Limestone is concentrated in fine fractions (<8 μm) while the clinker is concentrated in coarser ones. However, limestone content over 30% obstructs the grinding of both clinker and limestone [323].

Also calcinate formed during the processing of strontium aluminate clinker must be finely ground in order to prepare the strontium aluminate cement. The increase in specific surface area improves the reactivity of binder with water. Moreover, the admixtures such as cal‐ cined bauxite and alumina can be introduced into the clinker. These mineral admixtures serve as micro-fillers, similarly to calcite4 milled with clinker during the preparation of Port‐ land cement [315,320,323,324]. The grinding kinetics, the effect of grinding media and the additives were already described in Chapter 2.7.

The procedure is divided into two sequential phases; crushing of lumps (3 – 25 mm) into loosely connected wafers in a dry roller press and subsequent fine milling of pre-processed clinker

94 Strontium Aluminate - Cement Fundamentals, Manufacturing, Hydration, Setting Behaviour and Applications

As was mentioned above, the ball mill is commonly used for fine milling of cement clinkers. The type of grinding media exerts significant influence on milling performance in terms of the product size and energy consumption. Various shapes of grinding media including rods, pebbles, and cylinders are used as an alternative to balls. The cylinders received particular attention because they have a greater surface area and higher bulk density than balls of similar

Grinding of clinker represents energetically demanding part of the production process, which consumes about one-third of energy needed to produce cement. The production of fine ground clinker requires grinding stabilizers (grinding activators) which prevent the clinker from reagglomeration. Such additives, which are well known in both dry grinding and wet grinding processes, help decrease the enormous energy consumption of cement production

For most of the twentieth century, the dry grinding circuits for the production of finished cement from cement clinker which consist of two-compartment tube mills and air separators, have been used. It is not uncommon to produce cement in an open circuit. The advances in cement grinding technology are slow and limited to more developed countries. Approximately 95% of feed to the cement grinding circuit are clinker and the rest of feed are ''additives'' which include grinding aids. The quality of cement is measured by the surface area or the Blaine

permeability test. In the past 20 years, high pressure grinding roll (HPGR) technology has been used in pre-crushing the clinker. Presently, many American and European cement grinding circuits have HPGR which increases the grinding capacity and energy efficiency [279].

The effectiveness of seven grinding aids, namely triethanolamine, mono-and diethylene glycols, oleic acid, sodium oleate, sulphite waste liquor and dodecylbenzene sulphonic acid on the batch grinding of Portland cement clinker, limestone and quartz was investigated in a laboratory ball mill by Sohoni at al. [322]. While the grinding aids had only a marginal effect on grinding of quartz, they had significantly beneficial effect on the grinding of limestone and cement clinker. Triethanolamine appeared to be the most effective of all aids studied. In grinding of cement clinker, gypsum also acted as very effective grinding aid. The action of these additives was attributed to their ability to prevent the agglomeration and balls and mill

The presence of easily ground limestone leads to a wider particle size distribution of mixture. Limestone is concentrated in fine fractions (<8 μm) while the clinker is concentrated in coarser ones. However, limestone content over 30% obstructs the grinding of both clinker and

Also calcinate formed during the processing of strontium aluminate clinker must be finely ground in order to prepare the strontium aluminate cement. The increase in specific surface area improves the reactivity of binder with water. Moreover, the admixtures such as cal‐

/kg, and this index is determined by the Blaine air

wafers in a rotating ball mill [316].

index. The unit of the Blaine index is m2

from coating by powder.

limestone [323].

mass and size [317-320].

[285,313,321].

<sup>4</sup> The use of Portland limestone cements has many benefits, both technical and economical. The European Prestandard prEN 197-1 identifies two types of Portland limestone cement containing 6–20% limestone and 21–35% limestone, respectively [320].

**Chapter 4**

**Processes during Thermal Treatment**

and pure carbonates (d).

The processes discussed in this chapter include the mechanisms and temperature ranges of chemical reactions and phase transformations, which take place during the treatment of strontium aluminate raw materials as the mixture of strontium carbonate and alumina. Fig.1 shows the equilibrium phase composition during the preparation of calcium (a), strontium (b) and barium aluminate clinker (c). These systems show many similarities, therefore alumina react with carbonate in the molar ratio close to one. Therefore, is interesting to compare the changes of equilibrium composition which take place with increasing temperature for clinkers

**Figure 1.** Calculated equilibrium composition during the thermal treatment of calcium (a), strontium (b) and barium

© 2014 The Author(s). Licensee InTech. This chapter is distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/3.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

aluminate cement (c) and thermal decomposition of pure carbonates (d).
